Materials and Design 29 (2008) Delamination in FRP laminates with holes under transverse impact. Tarapada Roy, Debabrata Chakraborty *


 Shanon Morris
 1 years ago
 Views:
Transcription
1 Materials and Design 9 (8) Materials & Design Delamination in FRP laminates with holes under transverse impact Tarapada Roy, Debabrata Chakraborty * Mechanical Engineering Department, Indian Institute of Technology Guwahati , Assam, India Received 4 July 6; accepted 14 November 6 Available online 16 January 7 Abstract The present paper deals with the study of hybridization on impact response and impact induced delamination of laminated composite plates with holes. Three dimensional finite element analysis has been done to evaluate the response of graphite/epoxy laminate as well as graphite/epoxy kevlar/epoxy hybrid laminate subjected to impact loading, and stress based delamination criterion has been used to assess the chances of delamination initiation from the inner edges of the hole at different interfaces. The present study concludes that incorporation of kevlar/epoxy at the outer layers of the [/ 45/45/9] S in the graphite/epoxy laminate improves the impact resistance of the laminate in terms of reduced magnitude of the contact force but the chances of impact induced delamination at the interfaces increase. Ó 6 Elsevier Ltd. All rights reserved. Keywords: Hybrid laminate; Finite element; Delamination; Contact impact 1. Introduction Inherent advantages like high specific weight and stiffness of fiber reinforced polymer (FRP) composites led to its extensive use in aerospace and allied industries. However, in spite of their having many advantages, the structures made of FRP composites are susceptible to transverse impact. Especially in the case of low velocity impact, damages such as matrix cracking, fiber breakage and delamination occur at certain specific plies in the laminate depending upon the stacking sequence as well as the strength of the plies leading to embedded defects which are not apparent. Many a times the laminated composite plates contain holes due to various reasons like accommodating bolted joints or other mating parts in the structures. The presence of such holes in a laminate gives rise to free edges around the inner circumference of the hole. Subjected to loading, interlaminar stresses develop at these free edges and delamination may initiate depending upon the strength of the interface. Once a defect of this kind occurs in a laminated structure, * Corresponding author. Tel.: ; fax: address: (D. Chakraborty). failure initiates from that location leading to the final fracture of the laminate. Many investigations have been performed to study the response of laminated composites under low velocity impact and the approaches to improve the impact resistance of laminated composites. Hybridization has been one of the ways to improve the impact resistance of the laminated composites. Experimental and numerical studies have been conducted to study the improvement of impact response of laminated composites by way of hybridization. Some of the important works in this direction are presented in the following paragraph. Sun and Chattopadhyay [1] investigated the impact of a mass on a simply supported composite plate under initial stress by solving a nonlinear integral equation and obtained the contact force and dynamic response of the plate. Sun and Chen [] analyzed the impact response behavior of initially stressed composite plate. Wu et al. [3] performed a transient dynamic finite element analysis of a laminated FRP plate subjected to the impact of foreign object and presented the stress and strain distribution through the thickness during impact. Choi and Chang [4] studied the impact damage on graphite/epoxy laminated composites caused by a low velocity impact in terms of /$  see front matter Ó 6 Elsevier Ltd. All rights reserved. doi:1.116/j.matdes
2 T. Roy, D. Chakraborty / Materials and Design 9 (8) matrix cracking and delamination resulting from a point node impact. Lam and Sathiyamoorthy [5] presented a theoretical method to analyze the impact dynamics of a system, which consists of laminated beam, subjected to the impact of multiple spherical masses. Duan and Ye [6] developed a 3D finite element model incorporating frictional contact for studying the delamination at the interfaces due to low velocity impact. Li et al. [7] investigated the effect of plate size, boundary condition, impactor mass and velocity on delamination size. Tay et al. [8] applied element failure concepts for dynamic fracture and delamination in the low velocity impact of composites. Alsan et al. [9] conducted experiments and performed 3D finite element analysis to evaluate the delamination damage of Eglass/epoxy laminated composites subjected to low velocity impact and evaluated the delamination at various interfaces. Shyr and Pan [1] investigated the damage characteristics and failure strengths of composite laminates at low velocity impact by performing experiments using a guided drop weight test rig and observed that the fiber breakage had occurred prior to the major damage. Moura and Goncalves [11] modelled the interaction between matrix cracking and delamination in carbon epoxy laminates under low velocity impact. They developed a numerical model based on an interface finite element compatible with 3D solid elements. Choi and Lim [1] suggested that linearized contact law could be well applied to low velocity impact analysis of composite laminates. Tay and Gosse [13] reported the use of element failure concepts with a recent failure criterion called the strain invariant failure theory (SIFT) in the direction of damage progression in a composite laminate subjected to threepoint bend. Zou et al. [14] proposed a method for modeling the damage of multiple delaminations and transverse matrix cracking in laminated composites due to low velocity lateral impact. Allix and Blanchard [15] analyzed the mesomodelling of delamination towards industrial applications and presented a structural failure criterion in order to predict which levels of damage and delamination are critical. Hosseizadeh et al. [16] analyzed the damage behavior of fiber reinforced composite plates subjected to drop weight impacts. In the direction of improving the impact response by hybridization, Adams and Zimerman [17] showed that the impact performance of graphite/epoxy laminate could be improved by hybridization with discrete plies of polyethylene/epoxy. Jang et al. [18] showed that addition of nylon/epoxy, polyester/epoxy and polyethylene/epoxy led to improvement of impact resistance of graphite/epoxy according to stacking sequence. Lee et al. [19] studied the effect of hybridizing graphite/epoxy with glass/epoxy and kevlar/epoxy on the impact resistance. Literature review reveals that many works have already been done in the area of impact response of laminated composite structures and it still remains an important area of research. Hybrid laminates have been studied by many researchers for improvement of impact resistance of laminated composite structures. Laminated plates containing holes or cutouts have been studied very extensively in the literature [3 5]. However, most of these studies concentrated on tensile and compressive loading. Relatively fewer studies have been conducted on the impact failure of composite plates containing holes or cutouts. Composite plates containing holes are more prone to delamination initiating at the interface near the edges of the holes. Therefore, the present paper aims at studying the response of the single and hybrid laminated composite plates with holes due to low velocity impact and also studying the chances of delamination at the interfaces of such laminates.. Finite element formulation Fig. 1 shows a laminated FRP composite plate of length L, width W and thickness h consisting of N laminae of different fiber orientation, clamped at its four edges and impacted by a spherical impactor of mass m and striking with an initial velocity of V Noded layered solid element Threedimensional 8noded isoparametric layered solid elements were used for modeling of the laminated plate (Fig. ). The shape functions defining the geometry and displacement are N i ¼ 1 8 ð1 þ rr iþð1 þ ss i Þð1 þ tt i Þ; i ¼ 1; ; 3;...; 8 ð1þ where r, s, t are natural coordinates and r i, s i, t i are the values of natural coordinates for the ith node. Extra shape functions are introduced to the general 8noded solid element in order to simulate the flexural response and they are P 1 ¼ð1 r Þ P ¼ð1 s Þ P 3 ¼ð1 t Þ ðþ The displacement variation within the element is thus Fig. 1. Impact on a laminated plate with holes by spherical impactor.
3 16 T. Roy, D. Chakraborty / Materials and Design 9 (8) Gauss quadrature scheme is applied to evaluate the above integration. The stiffness matrix of Eq. (8) is reduced to 4 4 using static condensation technique. Element mass matrix is evaluated as Z ½M e Š¼ ½NŠ T q½nšdv ð9þ V m.. Contact impact modeling 8 9 >< u >= fdg ¼ v >: >; ¼ X8 w i¼1 N i 8 >< u i v i >: w 9 >= þ½pšfwg ð3þ >; where 3 P 1 P P ½PŠ ¼4 P 1 P P 3 5 P 1 P P 3 and ½WŠ T ¼ ½W 1 W W 3 W 4 W 5 W 6 W 7 W 8 W 9 Š The stiffness matrix is calculated as ½KŠ ¼ Let Z 1 Z 1 Z 1 Gðr; s; tþ ¼½BŠ T ½CŠ½BŠjJj then ½KŠ ¼ Z 1 Z 1 Z 1 ½BŠ T ½CŠ½BŠjJjdr dsdt Gðr; s; tþdr dsdt For an element having N layers in the thickness direction (Fig. ), T ¼ XN k¼1 t k Fig.. 8noded layered element. where T is the total thickness of the element and t k is the thickness of the kth layer of the element. Taking a parameter te[,t] and changing the limits ½KŠ ¼ Z 1 Z 1 X N Z t k t 1 k Gðr; s; tþdr dsdt ð8þ T k¼1 where t is function of thickness over the layer. ð4þ ð5þ ð6þ ð7þ Dynamic equation governing the impact problem (neglecting damping) at time t + Dt is ½MŠf dg tþdt þ½kšfdg tþdt ¼fFg tþdt ð1þ where [M] and [K] are the mass and stiffness matrices and ff g; fdg; f dg; _ f dg are force, displacement, velocity and acceleration vectors for plate, respectively, at time t + Dt. Using Newmarkb method, Eq. (1) can be reduced to ½ bkšfdg tþdt ¼fbF g tþdt ð11þ where ½ bkš is the effective stiffness matrix and ½bF Š is the effective force vector and are defined as ½ bkš ¼ 1 UDt ½MŠþ½KŠ fbf g¼fhg t þffg tþdt fhg t 1 ¼½MŠ UDt fdgt þ 1 UDt f dgþ _ 1 U 1 f dg ð1þ ð13þ ð14þ where / and d are the Newmark constants. In Eq. (11), displacement, velocity and acceleration at time t are known at each point inside the plate and the unknown quantities in this equation are vector {d} t+dt and the force vector {F} t+dt. In the absence of preload, (11) becomes ½ bkšfdg tþdt ¼fHg t þfpg tþdt ð15þ where {P} is the contact force. The displacement vector {d} is expressed as the sum of the displacements due to the force {H} and the contact force {P} as fdg tþdt ¼fdg tþdt H þfdg tþdt P Eqs. (15) and (16) give ð16þ ½ bkšfdg tþdt H ¼fHg t ð17þ and ½ bkšfdg tþdt P ¼fPg tþdt ð18þ Writing {P} t+dt = f t+dt {U}, where f t+dt is the magnitude of contact force at time t + Dt, Eq. (18) yields ½ bkšfdg tþdt P ¼ f tþdt fug ð19þ and for a unit contact force (f t+dt =1)
4 T. Roy, D. Chakraborty / Materials and Design 9 (8) ½ bk Šfdg tþdt U ¼fUg ðþ where fdg tþdt U is the displacement caused by the unit contact force and d tþdt C ¼ d tþdt CH þ f tþdt d tþdt CU ð7þ Combining Eqs. () (7), the following expressions for the contact force are obtained: Z tþdt Z tþdt Z tþdt 1:5 f tþdt f ¼ j vdt þ dt dt dtþdt CH m f tþdt d tþdt CU during loading f tþdt ¼ f m R tþdt vdt þ R tþdt R tþdt f dt dt dtþdt m CH f tþdt d tþdt CU a a m a! :5 during unloading ð8þ fdg tþdt P ¼ f tþdt fdg tþdt U Eqs. (16) and (1) give fdg tþdt ¼fdg tþdt H þ f tþdt fdg tþdt U ð1þ ðþ Using Hertzian contact law, contact forces during loading and unloading are f tþdt ¼ jða tþdt Þ 1:5 during loading :5 during unloading f tþdt ¼ f m a tþdt a a m a ð3þ where j is the modified constant of the Hertz contact theory, a is the indentation depth, f m is the maximum force just before unloading, a m is the indentation depth corresponding to f m and a is the permanent indentation during loading and unloading process. Permanent indentation can be determined from the following expressions: a ¼ when a m < a cr " a ¼ a m 1 a # =5 cr ð4þ when a m > a cr a m Contact force at t + Dt, i.e. f t+dt, was calculated using Eq. (8) (during loading or during unloading) by Newton Raphson method. From the known value of contact force f t+dt, displacement vector {d} t+dt is calculated using Eq. (). Once the value of f t+dt is known, plate velocity, acceleration and then the stresses and strains at time t + Dt were calculated. This procedure has been repeated for each time step to get the displacement, stress and strain. The nodal stresses are obtained by using a leastsquare formulation proposed by Hinton and Campbell []. The extrapolated nodal stresses are obtained by ðr i Þ¼½ST Šðr J Þ ð9þ where r i and r j are nodal and Gauss point stresses, respectively, [ST] is the transformation matrix. For the present analysis, the transformation matrix from Gaussian stresses to extrapolated nodal stresses for threedimensional eight nodded layered brick element is obtained by ½ST Š¼ N 1 ðr j ; s j ; t j ÞN 1 ðr j ; s j ; t j Þ : : N 1 ðr j ; s j ; t j ÞN 8 ðr j ; s j ; t j Þ N ðr j ; s j ; t j ÞN 1 ðr j ; s j ; t j Þ : : N ðr j ; s j ; t j ÞN 8 ðr j ; s j ; t j Þ... : : N 8 ðr j ; s j ; t j ÞN 1 ðr j ; s j ; t j Þ : : N 8 ðr j ; s j ; t j ÞN 8 ðr j ; s j ; t j Þ 3 N 1 ðr I ; s I ; t I Þ : : N 1 ðr VIII ; s VIII ; t VIII Þ... : : : :... 5 N 8 ðr I ; s I ; t I Þ : : N 8 ðr VIII ; s VIII ; t VIII Þ where a cr is the critical indentation. a tþdt ¼ d tþdt S Here d tþdt S and d tþdt C d tþdt C ð5þ is the position of the center point of the impactor is the displacement of the center of the mid surface of the plate in the direction of impact. At time t + Dt, the magnitude of d tþdt S can be determined by Newton s second law as d tþdt S ¼ Z tþdt vdt þ Using Eq. (), we have Z tþdt Z tþdt f dt dt m ð6þ where VIII is the number of Gauss points..3. Delamination at the interface In order to assess delamination initiation at the interface, the criterion proposed by Choi et al. [1] for impact induced delamination has been used in the present work. The criterion is D a r n 4 yz þ rnþ1 S n i xz S nþ1 i! þ rnþ1 yy Y nþ1! 3 5 ¼ e D ð3þ
5 18 T. Roy, D. Chakraborty / Materials and Design 9 (8) if e D P 1 failure e D 6 1 no failure Y n ¼ Y n ten if r yy P Y n ¼ Y n c if r yy 6 where D a is an empirical constant which has to be determined from the experiment, which has been taken as 1.8 as suggested by Choi et al. [4]. r xz is averaged interlaminar stress within the nth interface, which can be expressed as r n xz ¼ 1 h n Z tn t n r xz dt where t n and t n are upper and lower interfaces of nth ply in the laminate and h n is the thickness of the ply. 3. Results and discussion 3.1. Validation Based on the contact impact finite element formulation above, a computer code has been developed in C language for the present study. In order to verify the FE code developed, the following parameters were used for a steel ball impacting at the center of an isotropic plate. Plate dimensions:...8 m 3 with the four edges clamped; Impactor (steel ball) diameter:. m; Velocity of the impactor: 1 m/s; Steel properties: E = 1 9 N/m, G = N/m, t =.5, a cr =.1 m, density = 784 Kg/m 3. It has been observed that for a mesh size of (8 elements), and a time step of Dt = 1ls, an excellent agreement has been achieved with the analytical solution of Karas []. This is shown in Fig. 3. The code has also been validated for the impact of aluminum sphere on a [/ 45/45/9] S graphite/epoxy laminate, and excellent agreement on contact force, displacements, velocities of plate and impactor has been obtained with already published results of Wu and Chang [3]. Fig. 4 only shows the contact force history of such a graphite/epoxy laminate. Fig. 4. Contact force using present code with mesh size for impact of aluminum sphere on [/ 45/+45/9] S. 3.. Transverse impact on a laminate with holes A square laminated composite plate of length and width equal to 8 mm and thickness of 3 mm has been considered in the present study. The plate contains two circular holes of 4 mm diameter and is symmetrically placed with respect to the center of the plate. The centertocenter distance of the holes is mm. Threedimensional 8noded layered elements have been used to model the plate with fine refinement near the holes. Fig. 5 shows the template of a typical 3D FE mesh of the above model. Total number of elements in the FE model were 18 and the number of nodes was 919. Three types of laminates have been analyzed to assess their comparative performance in terms of impact response as well as the impact induced delamination at the interface. In the present case, [/ 45/45/9] S laminate has been considered. The laminate actually consists of four sub laminates each having a stacking sequence of [/ 45/45/9]. Three different laminates viz. GGGG, KGGK1 and KGGK have been analyzed to study their impact responses and the effect of hybridization on the impact response. Here, GGGG stands for [ G /45 G /45 G /9 G ] S, KGGK1 stands for [ K / 45 G /45 G /9 G / G / 45 G /45 G /9 G ] S and KGGK indicates [ K / 45 K /45 K /9 K / G / 45 G /45 G /9 G ] S where K and Fig. 3. Contact force compared with Karas solution [] with mesh size. Fig. 5. Template of 3D FE mesh of the plate with holes.
6 T. Roy, D. Chakraborty / Materials and Design 9 (8) Table 1 Materials properties for graphite/epoxy and kevlar/epoxy Lamina material property Graphite/ epoxy (G) Aramid/ epoxy (K) Critical indentation, a cr 8.64e 5 m 1.16e 4 m Longitudinal Young s 181 GPa 76 GPa modulus, E xx Transverse Young s modulus, E yy 1.3 GPa 5.5 GPa Shear modulus in x y 7.17 GPa.3 GPa direction, G xy Poisson s ratio in x y direction,.8.34 t xy Poisson s ratio in y z direction, t yz.8.34 Density 16 kg/m kg/m 3 Allowable longitudinal tensile 15 MPa 14 MPa stress, X t Allowable longitudinal 15 MPa 35 MPa compressive stress, X c Allowable transverse tensile 4 MPa 1 MPa stress, Y t Allowable transverse compressive 46 MPa 53 MPa stress, Y c Allowable inplane shear stress, S i 68 MPa 34 MPa Contact coeficient, j e8 N m e8 N m.5 G stand for kevlar/epoxy and graphite/epoxy lamina, respectively. The laminate is assumed to be clamped along all the four edges and impacted at the center by a 1.7 mm diameter aluminum sphere at a velocity of 9 m/s. The material properties used for the above calculations are listed in Table 1. Fig. 6 shows the contact force history for different laminates when impacted by the spherical aluminum impactor at 9 m/s. It could be clearly observed from this figure that magnitude of contact force is maximum for GGGG laminate while it is minimum for KGGK laminate. Contact force magnitude for KGGK1 hybrid laminate lies in between. It could also be observed that even though reloading occurs for all the three types of laminates, contact duration is much less in the case of graphite/epoxy laminate (GGGG) compared to that in the case of other two laminates. So, introduction of kevlar/epoxy increases the flexibility of the laminate compared to graphite/epoxy Fig. 7. Comparison of plate displacement for different laminates at 9 m/s impact velocity. Fig. 8. Comparison of impactor displacement for different laminates at 9 m/s impact velocity. laminates. Fig. 7 shows the plate displacement and as expected plate displacement is minimum in the case of graphite/epoxy (GGGG) and increases with the inclusion of kevlar/epoxy plies in the laminates. Fig. 8 shows the impactor displacement history and in consistent with contact force, rebound is maximum in case of graphite/epoxy. Impactor velocity history is shown in Fig. 9. Fig. 6. Comparison of contact force for different laminates at 9 m/s impact velocity. Fig. 9. Comparison of impactor velocity for different laminates at 9 m/s impact velocity.
7 13 T. Roy, D. Chakraborty / Materials and Design 9 (8) Fig. 1. Delamination size in the interfaces of single laminated plate (GGGG). Fig. 11. Delamination size in the interfaces of hybrid laminated plate (KGGK1).
8 T. Roy, D. Chakraborty / Materials and Design 9 (8) Using the stress based delamination criterion, delaminations at the interfaces have been assessed for different laminates subjected to the impact of aluminum sphere at 9 m/s. Fig. 1 shows that after 6 ls, delaminations occur only at three interfaces in the case of GGGG laminate. Fig. 11 shows that after 6 ls, delaminations occur only at four Fig. 1. Delamination size in the interfaces of hybrid laminated plate (KGGK).
9 13 T. Roy, D. Chakraborty / Materials and Design 9 (8) interfaces in the case of KGGK1 laminate. Fig. 1 shows that delaminations occur at as many as seven interfaces in case of KGGK laminate. The extent of delamination at a particular interface is highest in the case of KGGK laminate and lowest in the case of GGGG laminate and in the case of KGGK1 the extent of delamination is in between. The reason for more delaminations in case of KGGK1 and KGGK laminates compared to GGGG laminate is that the interfacial shear and normal strengths of graphite/epoxy is higher compared to that of kevlar/epoxy. Thus even though providing a kevlar/epoxy at the outer layer prevents the laminate from failure at the contact point due to low magnitude of contact force and contact stress, chances of delamination at the interface increase. From Figs. 1 1 which show delaminations at the interface of the laminates, it is clear that due to the presence of holes in the laminate, delaminations initiate from the vicinity of holes at different interfaces. It could also be observed that delamination propagates from the inner edges of holes towards impact point and from outer edges towards the edges of the plate with some specific direction. The direction of delamination at interfaces 1 and follows the direction of fiber in the ply below the interface, which agrees with already published observations. It could be observed from the figures that in the case of GGGG and KGGK1, delaminations occur only at the tensile side of the plate but in the case of KGGK, delamaninations occur also at the interfaces located in the compression side of the plate showing that the interfaces in the KGGK are more susceptible to delamination under impact loading. 4. Conclusions Threedimensional transient dynamic finite element analysis has been done to analyze the response of single material (graphite/epoxy) and hybrid (graphite/epoxy kevlar/epoxy) laminates having holes in it. Stress based delamination criterion has been used to assess the chances of impact induced delamination from the vicinity of the holes. From the present study, it is quite clear that delaminations initiate at the interface from the inner free edges of the holes and with time, delaminations from two holes meet each other forming a big delamination area. It is evident from the present study that kevlar/epoxy graphite/epoxy hybrid laminate is more flexible compared to only graphite/epoxy laminates. Even though kevlar/epoxy hybridization on graphite/epoxy laminate leads to reduced contact force and hence more impact resistance in terms of failure due to contact stresses, but the chances of delamination at the interfaces increase. References [1] Sun CT, Chattopadhyay S. Dynamic response of anisotropic laminated plates under initial stress to impact of a mass. J Appl Mech 1975;4: [] Sun CT, Chen JK. On the impact of initially stressed composite laminates. J Compos Mater 1985;19: [3] Wu H, Yung T, Chang FK. Transient dynamic analysis of laminated composite plate subjected to transverse impact. Comput Struct 1989;31: [4] Choi HY, Chang FK. A model for predicting damage in graphite/ epoxy laminated composite resulting from lowvelocity impact. J Compos Mater 199;6(14): [5] Lam KY, Sathiyamoorthy TS. Response composite beams under low velocity impact of multiple masses. Compos Struct 1999;44:5. [6] Duan SH, Ye TQ. Three dimensional frictional dynamic contact analysis for predicting low velocity impact damage in composites. Adv Eng Software ;33:9 15. [7] Li CF, Hu N, Cheng JG, Fukunaga H, Sekine H. Lowvelocity impactinduced damage of continuous fiberreinforced composites laminates. Part II. Verification and numerical investigation. Compos Part A ;33: [8] Tay TE, Tan VBC, Deng M. Elementfailure concepts for dynamic fracture and delamination in lowvelocity impact of composites. Int J Solids Struct 3;4: [9] Alsan Z, Karakuzu R, Okutan B. Response of laminated composite plates under low velocity impact loading. Compos Struct 3;59: [1] Shyr TW, Pan YH. Impact resistance and damage characteristics of composite laminates. Compos Struct 3;6: [11] Moura MFSF, Goncalves JPM. Modelling the interaction between matrix cracking and delamination in carbon epoxy laminates under low velocity impact. Compos Sci Technol 4;64:11 7. [1] Choi IH, Lim CH. Low velocity impact analysis of composite laminates using linearized contact law. Compos Struct 4;66: [13] Tay TE, Tan SHN, Tan VBC, Gosse JH. Damage progression by the elementfailure method (EFM) and strain invariant failure theory (SIFT). Compos Sci Technol 5;65: [14] Li S, Reid SR, Zou Z. Modelling damage of multiple delaminations and transverse matrix cracking in laminated composites due to low velocity lateral impact. Compos Sci Technol 6;66: [15] Allix O, Blanchard L. Mesomodelling of delamination: towards industrial applications. Compos Sci Technol 6;66: [16] Hosseinzdeh R, Shokrieh MM, Lessard L. Damage behavior of reinforced composite plates subjected to drop weight impacts. Compos Sci Technol 6;66:61 8. [17] Adams DF, Zimmerman RS. Static and impact performance of polyethylene fiber/graphite hybrid composites. SAMPE J. 1986;:1 6. [18] Jang BZ, Chen LC, Wang CZ, Lin HT, Zee RH. Impact resistance and energy absorption mechanism in hybrid composites. Compos Sci Technol 1989;34: [19] Lee YShin, Kang KHee, Park O. Response of hybrid laminated composite plates under lowvelocity impact. Compos Struct 1997;65: [] Hinton E, Champbell JS. Local and global smoothing of discontinuous finite element functions using a least squares method. Int J Numer Meth Eng 1974;8: [1] Choi HY, HisYoung TW, Chang FK. A new approach towards understanding damage mechanism and mechanics of laminated composites due to low velocity impact: Part II analysis. J Compos Mater 1991;5: [] Karas K. Platten Unter Seitchem stoss. Ing Arch 1939;1:37 5. [3] Awerbuch JA, Madhukar MS. Notched strength of composite laminate: prediction and experiments a review. J Reinf Plast Comp 1985;4: [4] Chang FK, Chang KY. Post failure analysis of Bolted Composite joints in tension or shearout mode failure. J Compos Mater 1987;1: [5] Chang FK, Lessard LB. Damage tolerance of laminated composites containing an open hole and subjected to compressive loadings: Part I analysis. J Compos Mater 1991;5:3 43.
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationA Numerical Study on Prediction of BFS in Composite Structures under Ballistic Impact
VOL. 1, 2015 ISSN 2394 3750 EISSN 2394 3769 SCIENCE & TECHNOLOGY A Numerical Study on Prediction of BFS in Composite Structures under Ballistic Impact Bandaru Aswani Kumar 1, Suhail Ahmad 2 1. Research
More informationProgressive Damage of GFRP Composite Plate Under Ballistic Impact: Experimental and Numerical Study
Progressive Damage of GFRP Composite Plate Under Ballistic Impact: Experimental and Numerical Study Progressive Damage of GFRP Composite Plate Under Ballistic Impact: Experimental and Numerical Study Md
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationNumerical Analysis of Delamination Behavior in Laminated Composite with Double Delaminations Embedded in Different Depth Positions
Numerical Analysis of Delamination Behavior in Laminated Composite with Double Delaminations Embedded in Different Depth Positions Numerical Analysis of Delamination Behavior in Laminated Composite with
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationEffect Of Multiple Delamination on Composite Turbine Blade Subjected to Low Velocity Impact
Effect Of Multiple Delamination on Composite Turbine Blade Subjected to Low Velocity Impact Sudip Dey* Mechanical Engineering Department, Jadavpur University Kolkata 700032, INDIA * Email of corresponding
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationCapability Assessment of Finite Element Software in Predicting the Last Ply Failure of Composite Laminates
Available online at www.sciencedirect.com Procedia Engineering 41 (2012 ) 1647 1653 International Symposium on Robotics and Intelligent Sensors 2012 (IRIS 2012) Capability Assessment of Finite Element
More informationSSRG International Journal of Mechanical Engineering (SSRGIJME) volume1 issue5 September 2014
Finite Element Modeling for Delamination Analysis of Double Cantilever Beam Specimen Mohammed Waseem H.S. 1, Kiran Kumar N. 2 1 Post Graduate Student, 2 Asst. Professor Dept. of Mechanical Engineering,
More informationDynamic Response Of Laminated Composite Shells Subjected To Impulsive Loads
IOSR Journal of Mechanical and Civil Engineering (IOSRJMCE) eissn: 22781684,pISSN: 2320334X, Volume 14, Issue 3 Ver. I (May.  June. 2017), PP 108123 www.iosrjournals.org Dynamic Response Of Laminated
More informationCOMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS COMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES Hiroshi Suemasu*, Wataru Sasaki**, Yuuichiro Aoki***, Takashi Ishikawa**** *Department of
More informationTransient dynamic response of delaminated composite rotating shallow shells subjected to impact
Shock and Vibration 13 (2006) 619 628 619 IOS Press Transient dynamic response of delaminated composite rotating shallow shells subjected to impact Amit Karmakar a, and Kikuo Kishimoto b a Mechanical Engineering
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationEffect of magnetostrictive material layer on the stress and deformation behaviour of laminated structure
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Effect of magnetostrictive material layer on the stress and deformation behaviour of laminated structure To cite this article:
More informationDynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load
Dynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load Arun Mukherjee 1, Dr. Sreyashi Das (nee Pal) 2 and Dr. A. Guha Niyogi 3 1 PG student, 2 Asst. Professor,
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationNonlinear constitutive models for FRP composites using artificial neural networks
Mechanics of Materials 39 (2007) 1035 1042 www.elsevier.com/locate/mechmat Nonlinear constitutive models for FRP composites using artificial neural networks Rami HajAli *, HoanKee Kim School of Civil
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationIndentation Energy in Bending of Sandwich Beams with Composite Laminated Faces and Foam Core
Indentation Energy in Bending of Sandwich Beams with Composite Laminated Faces and Foam Core M. SADIGHI, H. POURIAYEVALI, and M. SAADATI Dept. of Mechanical Engineering, Amirkabir University of Tech, Tehran,
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationProbabilistic fatigue life prediction of multidirectional composite laminates
Composite Structures 69 () 9 www.elsevier.com/locate/compstruct Probabilistic fatigue life prediction of multidirectional composite laminates Yongming Liu, Sankaran Mahadevan * Department of Civil and
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationFailure modes of glass panels subjected to soft missile impact
Failure modes of glass panels subjected to soft missile impact L. R. Dharani & J. Yu Dept. of Mech. and Aerospace Engineering and Engineering Mechanics, University of MissouriRolla, U.S.A. Abstract Damage
More informationEQUIVALENT FRACTURE ENERGY CONCEPT FOR DYNAMIC RESPONSE ANALYSIS OF PROTOTYPE RC GIRDERS
EQUIVALENT FRACTURE ENERGY CONCEPT FOR DYNAMIC RESPONSE ANALYSIS OF PROTOTYPE RC GIRDERS Abdul Qadir Bhatti 1, Norimitsu Kishi 2 and Khaliq U Rehman Shad 3 1 Assistant Professor, Dept. of Structural Engineering,
More informationThermal loadinduced notch stress intensity factors derived from averaged strain energy density
Available online at www.sciencedirect.com Draft ScienceDirect Draft Draft Structural Integrity Procedia 00 (2016) 000 000 www.elsevier.com/locate/procedia 21st European Conference on Fracture, ECF21, 2024
More informationEFFECTIVENESS OF NANO LAYERS ON INTERLAMINAR STREESES OF COMPOSITE LAMINATE
International Journal of Mechanical Engineering and Technology (IJMET) Volume, Issue 1, January 217, pp. 15 2, Article ID: IJMET 1_2 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=&itype=1
More informationNUMERICAL AND EXPERIMENTAL ANALYSES OF MULTIPLE DELAMINATIONS IN CURVED COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS NUMERICAL AND EXPERIMENTAL ANALYSES OF MULTIPLE DELAMINATIONS IN CURVED COMPOSITE LAMINATES A. Baldi 1 *, A. Airoldi 1, P. Belotti 1, P. Bettini
More informationStress intensity factor analysis for an interface crack between dissimilar isotropic materials
Stress intensity factor analysis for an interface crack between dissimilar isotropic materials under thermal stress T. Ikeda* & C. T. Sun* I Chemical Engineering Group, Department of Materials Process
More informationAbstract. 1 Introduction
Contact analysis for the modelling of anchors in concrete structures H. Walter*, L. Baillet** & M. Brunet* *Laboratoire de Mecanique des Solides **Laboratoire de Mecanique des ContactsCNRS UMR 5514 Institut
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationBending Analysis of Symmetrically Laminated Plates
Leonardo Journal of Sciences ISSN 15830233 Issue 16, JanuaryJune 2010 p. 105116 Bending Analysis of Symmetrically Laminated Plates Bouazza MOKHTAR 1, Hammadi FODIL 2 and Khadir MOSTAPHA 2 1 Department
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationSPECTRAL FINITE ELEMENT METHOD
SPECTRAL FINITE ELEMENT METHOD Originally proposed by Patera in 1984 for problems in fluid dynamics Adopted for problems of propagation of acoustic and seismic waves Snapshot of the propagation of seismic
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationCFRP. FRP FRP. Abaqus
C Epoxy C baqus C FE baqus C amene.kia@gmail.com EROG 1 Debonding : / C (mm) E c (MPa) f' c (MPa) f' t (MPa) a S L d h b 1 2 3 1 2 3 baqus C Leong Kok Leong Kok CDP E p (GPa) (MPa) E a (MPa) G a (MPa)
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationTheoretical Approach to Predict Transverse Impact Response of VariableStiffness Curved Composite Plates
*Manuscript Click here to view linked References 1 1 1 1 1 1 1 0 1 0 1 0 1 0 1 0 1 Theoretical Approach to Predict Transverse Impact Response of VariableStiffness Curved Composite Plates B. Arachchige,
More informationNumerical Evaluation of Fracture in Woven Composites by Using Properties of Unidirectional Type for modelling
J. Basic. Appl. Sci. Res., 2(12)1320213209, 2012 2012, TextRoad Publication ISSN 20904304 Journal of Basic and Applied Scientific Research www.textroad.com Numerical Evaluation of Fracture in Woven Composites
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationEDEM DISCRETIZATION (Phase II) Normal Direction Structure Idealization Tangential Direction Pore spring Contact spring SPRING TYPES Inner edge Inner d
Institute of Industrial Science, University of Tokyo Bulletin of ERS, No. 48 (5) A TWOPHASE SIMPLIFIED COLLAPSE ANALYSIS OF RC BUILDINGS PHASE : SPRING NETWORK PHASE Shanthanu RAJASEKHARAN, Muneyoshi
More informationMechanical Properties of Fiber Reinforced Composites Using Buckminster Fullerene Reinforcement
IJRMET Vo l. 4, Is s u e Sp l  1, No v 2013 Ap r i l 2014 ISSN : 22495762 (Online ISSN : 22495770 (Print Mechanical Properties of Fiber Reinforced Composites Using Buckminster Fullerene Reinforcement
More informationNonlinear bending analysis of laminated composite stiffened plates
Nonlinear bending analysis of laminated composite stiffened plates * S.N.Patel 1) 1) Dept. of Civi Engineering, BITS Pilani, Pilani Campus, Pilani333031, (Raj), India 1) shuvendu@pilani.bitspilani.ac.in
More informationReliability analysis of different structure parameters of PCBA under drop impact
Journal of Physics: Conference Series PAPER OPEN ACCESS Reliability analysis of different structure parameters of PCBA under drop impact To cite this article: P S Liu et al 2018 J. Phys.: Conf. Ser. 986
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationBuckling analyses of composite laminate skew plates with material nonlinearity
Composites: Part B 7 (6) 6 6 www.elsevier.com/locate/compositesb Buckling analyses of composite laminate skew plates with material nonlinearity HsuanTeh Hu*, ChiaHao Yang, FuMing Lin Department of Civil
More informationCalibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques
9 th International LSDYNA Users Conference Optimization Calibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques Stefano Magistrali*, Marco
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationCOMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD
10th International DAAAM Baltic Conference "INDUSTRIAL ENGINEERING  1213 May 2015, Tallinn, Estonia COMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD Sedláček,
More informationFinite Element Simulation of BarPlate Friction Welded Joints Steel Product Subjected to Impact Loading
Finite Element Simulation of BarPlate Friction Welded Joints Steel Product Subjected to Impact Loading Yohanes, a,* Muftil Badri, a Panji Adino, a Dodi Sofyan Arief, a and Musthafa Akbar, a a) Department
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationThe University of Melbourne Engineering Mechanics
The University of Melbourne 436291 Engineering Mechanics Tutorial Four Poisson s Ratio and Axial Loading Part A (Introductory) 1. (Problem 922 from Hibbeler  Statics and Mechanics of Materials) A short
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More informationFinite Element Analysis of Graphite/Epoxy Composite Pressure Vessel
Journal of Materials Science and Chemical Engineering, 2017, 5, 1928 http://www.scirp.org/journal/msce ISSN Online: 23276053 ISSN Print: 23276045 Finite Element Analysis of Graphite/Epoxy Composite
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationNumerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure
Copyright c 007 ICCES ICCES, vol.1, no.3, pp.9398, 007 Numerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure C. Bisagni 1 Summary The research here
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More informationFinite element analysis of drilled holes in unidirectional composite laminates using failure theories
American Journal of Science and Technology 2014; 1(3): 101105 Published online May 30, 2014 (http://www.aascit.org/journal/ajst) Finite element analysis of drilled holes in unidirectional composite laminates
More informationBallistic impact behaviour of thick composites: Parametric studies
Ballistic impact behaviour of thick composites: Parametric studies N.K. Naik *, A.V. Doshi Aerospace Engineering Department, Indian Institute of Technology Bombay, Powai, Mumbai 400 076, India Abstract
More informationBallistic impact behaviour of woven fabric composites: Parametric studies
Ballistic impact behaviour of woven fabric composites: Parametric studies N.K. Naik, P. Shrirao, B.C.K. Reddy Aerospace Engineering Department, Indian Institute of Technology Bombay, Powai, Mumbai 400076,
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationComparison of LSDYNA and NISA in Solving Dynamic Pulse Buckling Problems in Laminated Composite Beams
9 th International LSDYNA Users Conference Simulation Technology (1) Comparison of LSDYNA and NISA in Solving Dynamic Pulse Buckling Problems in Laminated Composite Beams Haipeng Han and Farid Taheri
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationStress analysis of functionally graded discs under mechanical and thermal loads
Indian Journal of Engineering & Materials Sciences Vol. 8, April 0, pp. 8 Stress analysis of functionally graded discs under mechanical and thermal loads Hasan Çallioğlu, Metin Sayer* & Ersin Demir Department
More informationComparison with LowVelocity Impact and Quasistatic Indentation Testing of Foam Core Sandwich Composites
International Journal of Applied Physics and Mathematics, Vol. 2, No. 1, January 212 Comparison with LowVelocity Impact and Quasistatic Indentation Testing of Foam Core Sandwich Composites Yan Li, An
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationMATERIALS AND METHODS
Modelling the Nonlinear Shear Stress Strain Behavior of a Carbon Fabric Reinforced Polyphenylene Sulphide From Rail Shear and [(458,2458)] 4s Tensile Test Ives De Baere, Wim Van Paepegem, Joris Degrieck
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationNUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS
5 th European LSDYNA Users Conference Composites NUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS Kevin Brown 1, Richard Brooks, Nicholas Warrior School of Mechanical, Materials and
More informationVIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS
VIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS Mechanical Engineering Department, Indian Institute of Technology, New Delhi 110 016, India (Received 22 January 1992,
More information